# modern techniques in polymerization: 4582- techniques in polymerization: 4582-605 ......

Post on 20-Feb-2018

225 views

Embed Size (px)

TRANSCRIPT

Modern Techniques in Polymerization: 4582-605

Instructor: Jeff Pyun

Aspects of Step-Chain-Living Polymerizations

MW Evolution of Step vs. Chain Growth Polymerization

University of ArizonaChem 542B: Step-Growth Polymerization

Conversion

MW

Conversion

MW

Step Growth Evolution of MW Chain Growth Evolution of MW

Reaction of difunctional monomersWith complementary functional groups

(A2 + B2)

4-Elementary reactions (initiation, propagation,termination, transfer) of reactive monomer + initiator

(vinylic- -systems, strained rings)

High polymer formed only at very high conversion

High polymer formed at low conversion

Heteroatom backbonesC-C bonds for vinylic monomers,

Heteroatom backbones for cyclic monomers

Conversion

MW

Requirements for Step-Growth Polymerization

High monomer purityDifunctionalityStoichiometryQuantitative conversion of monomer to polymer!No side Reactions

99 +

High polymer formed only at very high conversion!!!High polymer formed only at very high conversion!!!

Step Growth/Condensation Polymerization

Monomer Functionality and Polymer Architecture

Step-Growth

Difunctional monomers: linear polymers

A2 + B2; AB monomers

multifunctional monomers: branched, network polymers

A3 + B2; A2 + B3; Ax + Bx -gelationAB2; ABx monomers: (hyper)branched

For multifunctional monomersOnset of gelation strongly dependenton functionality of crosslinkers

Chain-Growthmonofunctional monomers: linear polymers

Vinylic: styrene, acrylates

Di-, multifunctional monomers: Crosslinked-networks

Dimethacrylates, divinylbenzene

multifunctional initiators: In living processes with fastControlled initiation

Stars, branched polymers

Carothers Theory for Molar Mass Prediction in Step-Growth Polymerization

Xn Defined as number average degree of polymerization

No Number of molecules presentinitially at T = 0 (i.e., monomers)

N Number of molecules presentinitially at T = t(both polymer and monomers)

p Extent of reaction (fractional, 100% = 1.0)AND the probability that any functionalgroup has reacted (i.e., formed bonds)

p =# of functional groups that have reacted# of functional groups initially present

Xn =No

N(eq. 1)

p =No - N

No

No

N=

1

1 - p(eq. 2)

Combine (eqs.1&2)

Xn =1

1 - pCarothers Eq.

Theory applicable to polymerizations of:A2 + B2; AB, A2-with stoichiometric balance

Requires perfect stoichiometric balance; high MW only at very high conversion!

MW distributions for Step-GrowthCarothers theory only provides Xn, Mn average values, no MW distributions!

Flory developed statistical theory to derive both number and weightfraction distributions

Mole fraction distributions

Weight fraction distributions

P(x) = probability distribution = number fraction distribution = mole fxn distrib.probability of a molecule possessing x monomer units at some time = t and p,where p = extent of reactioni and probability of functional group reacted

P(x) # of polymers of Xn = x

total # of macromolecules

1000 total polymer chains10 trimeric moleculesP(trimer) = 0.010

W(x) total mass polymers of Xn = x

total mass of macromolecules

1000g polymer chains10g trimeric moleculesW(trimer) = 0.010

Most Probable Distributions: Number Fraction

p = extent of reaction and probability that functional groups have reactedp = probability of finding bonds between monomers

Probability of finding a monomer: P(1) = 1 - pProbability of finding a dimer: P(2) = p(1 p)

Probability of finding a trimer: P(3) = p2(1 p)

Probability of finding an x-mer: P(x) = px-1(1 p)

This type of MW distribution referred to as a most probable distributionor Flory-Schulz distribution

Most Probable Distribution (p = 0.5)

0

0.10.2

0.3

0.4

0.5

0.6

1 2 3 4 5 6 7 8 9 10

DP

P(x

)

Series1

P(x) decreases monotonically with DPCharacteristic of step-growth polym.

P(x) = px-1(1 p) is discrete distr.

P(x) = (1/Xn)e-x/Xn continuous form

Most Probable Distributions with Higher Conversion

Most Probable Distribution (p = 0.1)

0

0.2

0.4

0.6

0.8

1

1 2 3 4 5 6 7 8 9 10

DP

P(x

)

Series1

Most Probable Distribution (p = 0.5)

0

0.1

0.2

0.3

0.40.5

0.6

1 2 3 4 5 6 7 8 9 10

DP

P(x

)

Series1

Most Probable Distrbution (p =0.9)

0

0.02

0.04

0.06

0.08

0.1

0.12

1 8 15 22 29 36 43 50 57 64

DP

P(x

)

Series1

Most Probable Distribution (p = 0.999)

0

0.0002

0.0004

0.0006

0.0008

0.001

0.0012

1 37 73 109 145 181 217 253 289 325 361 397 433 469

DP

P(x

)

Most Probable Distributions: Weight FractionProbability Distribution-Mole Fraction Distribution

P(x) = px-1(1 p) P(x) = mole fraction =N

Nx Nx = total number of X-mers

N = total number of molecules(monomer & polym) at someTime = t

Nx = N (1 p) px-1However, N is cumbersome to determine

N = No (1 - p) No = total number of molecules at T = 0

Nx = No(1 p)2 px-1

W(x) total mass polymers of Xn = x

total mass of macromolecules

Nx(x Mo)

No Mo=

Mo = ave. MWof repeat unit

W(x) x Nx

No= = x (1 p)2 px-1 Other eq. which defines

Flory-Schulz Distribution!

Polydispersity in Step-Growth Polym.

Mn = P(x) Mx = x Mo (1 p) px-1rememberP(x) = (1 p) px-1

Mx = x Mo

x px-1 = (1 p)-2 when p < 1

Polydispersity = Mw/Mn index for MW distribution

Mn =Mo

(1 p)= Xn Mo

rememberXn = 1/(1 p)

Mw = W(x) Mx = x2 Mo (1 p)2 px-1

x2 px-1 = (1 + p)(1 p)-3 when p < 1

rememberW(x) = px-1 x(1 p)2

Mx = x Mo

(1 + p)Mw = Mo(1 p) Mn

Mw = 1 + p

~[CO(CH2)4CO-NH(CH2)6NH]n~

PolyesterDacron, Mylar

polycarbonate

PolyamideNylon 6,6 Polyaromatic amide

Kevlar

PolyurethaneSpandex

Examples of Step-Growth Polymers

Key Features of Step-Growth PolymersMore expensive than chain-growth poylmers

Improved mechanical propertiesWider range of optical, electronic magnetic properties

Cl

Ph

F2C CF2

CO2CH3

Examples of Monomers Chain-Growth Polymerization

Ethylene

Propylene

Vinyl chloride

Tetrafluoroethylene

Styrene

Methyl methacrylate

Isoprene

O

O

O

O

O

O

O

Ethylene oxide Norbornene

-Caprolactone Lactide

Definition and Criteria for Living Polymerizations

Time

Ln [M]o[M]

Monomer Conversion

MW

Low Initiation Efficiency

Definition: Chain polymerization thatproceeds in the absence of chain breakingprocesses (termination, transfer

Criteria*: (Quirk et al., Polym. Int. 1992, 27, 359)1) Polymerization proceeds until all monomer

consumed, further addition of monomerresults in chain extension

2) Number average MW (Mn, Xn) linear relationshipwith monomer conversion

3) # of initiator molecules = # of polymer chains,which is constant throughout reaction

4) DP = [M]o/[I]o x conversion5) Polymers of low polydispersity formed

Mw/Mn = 1 + 1/DPn6) Block Copolymers formed from sequential

monomer addition to living polymer chain7) Facile chain end functionalization8) Linearity of Ln([M]o/[M]) vs. time (constant #

of active centers

Controlled/Living Polymerizations

Living polymerization:a chain growth process without chain-breaking reactions (termination, transfer) Anionic, Insertion (ROMP)

Features: precise DPn ([M]/[I]o)Low polydispersityActive chain ends-BlocksControl of architectureStringent reaction conditions

Controlled/Living polymerization:a chain growth process with chain-breaking reactions Rpropagation >> Rtermination, Rtransfer Reversible deactivation

Features: precise DPn ([M]/[I]o)Low polydispersity*Active chain ends-BlocksControl of architecture

Free Radical Chemistry: 1990s Greater functional group toleranceRange of monomers

_ +Li

Controlled/Living PolymerizationsLiving Anionic Polymerization

Initiators: ex. organolithium compounds (sec-butyl lithium; n-butyl lithium)Grignard reagents, alkali bases

Monomers: ex. Styrenes, dienes, (meth)acrylates, pyridines, epoxides:Functional monomer require protecting groups; alkyl esters cannot be polym

Features: exquisite control of MW, block copolymers, low functional grouptolerance

Controlled Cationic PolymerizationInitiators: ex. Alkyl halides, acetates, inorganic/organic acids, water

Monomers: ex. Vinyl ethers, alkenes(butylene), styrene, cyclic ethersFunctional monomer require protecting groups; alkyl esters cannot be polym

Features: highly reactive cation species susceptible to chain transferControlled MW, block copolymers

Controlled Radical PolymerizationInitiators: ex. Alkyl halides, alkoxyamines, thioesters

Monomers: ex. (meth)acrylates, (meth)acrylamides, styrenes, acrylonitrile,Pyridines, dienes,

High functional group tolerance, widest scope of polymerizable monomers

Features: controlled MW, blcck copoylmers, functionality, bimolecular termination

Rin

g-O

pe

nin

g P

oly

me

rization

Recommended